Int. J. Electrochem. Sci., 11 (2016) 3542 - 3554
International Journal of
An Investigation of the Surface Characterization of Laser
Surface Remelted and Laser Beam Welded AISI 316L Stainless
Faculty of Natural Sciences and Engineering, Department of Mechanical Engineering, Gaziosmanpaşa University, Tokat, 60150, Turkey
E-mail: email@example.com, firstname.lastname@example.org
Received: 2 February 2016 / Accepted: 24 February 2016 / Published: 1 April 2016
In this study, AISI 316L austenitic steel was joined by CO2 laser beam welding method and the microhardness and the surface characteristics of joints were investigated. Also, surface modification was applied on the laser welded and non-welded samples by means of Nd:YAG laser source at laser power 50W, 100W, and 150W. The main materials and the welding seam surfaces of the laser welded samples on which no laser modification had been applied and the surfaces of the samples on which laser surface modification was applied were characterized via SEM, Elemental Mapping, atomic force microscope (AFM), and at the same time, the changes in their surface hardness were identified. As a results, it was identified that the main material surface and the welding seam region of the laser welded sample on which no surface modification had been implemented had less roughness (Ra) than the samples on which laser surface modification had been applied. It was observed that the highest surface roughness belonged to the laser welded sample on which surface modification was applied via 150W laser power. No significant change was observed in the hardness values.
Keywords: Laser beam welding, Laser remelting, Austenitic stainless steel, Surface topography.
The Fe-Cr-Ni alloys that contain minimum 10.5% chromium and maximum 1.2% carbon in their chemical compositions are called stainless steel . When nickel is more than 8% in the stainless steel, which is classified into five categories according to its microstructures, makes austenite stable at room temperature, and this type of stainless steel is called austenitic stainless steel . This steel has high mechanical properties and corrosion resistance [3-6].
steel against pitting, 2% Mo is added to the alloy, and it is AISI 316L austenitic stainless steel that contains 17-19% chromium and 12-14% nickel; it is used especially in orthopaedic applications and in many branches of the industry . AISI 316L stainless steel is used in many branches of the industry since it has a good combination in terms of its mechanical characteristics, corrosion resistance, and capacity to be welded . The thin and protective chromium oxide layer that forms on the surface of AISI 316L stainless steel leads to corrosion resistance and biocompatibility [7-9]. Since it has high mechanical strength, good corrosion resistance, and is economical, it is commonly used in cardiovascular stents, orthodontic wires , and orthopaedic implants [10-12].
Studies that are designed to change the chemistry and physical topography of implant surfaces in order to extend the period of use of the biomedical implants such as AISI 316L stainless steel, and to improve their biocompatibility and osseointegration characteristics [8,13]. One other technique used for surface modification is laser surface remelting. As a result of the quick remelting-solidification that takes place on the surface with by means of the laser surface remelting modification procedure, surface hardness increases, abrasion and corrosion properties improve, a homogeneous surface structure forms, and, at the same time, as a result of an increase in the surface roughness, it results in a positive effect in the implant-tissue interface. In addition to medical field applications, laser surface modification is utilized since it improves the corrosion and abrasion resistance of structural materials [8,13-21]. Laser surface modification is a good choice for improving the resistance against cavitation erosion, pitting corrosion and intergranular corrosion, improvement in internal strains of austenitic stainless steels . After laser surface treatment, the treated surface becomes more resistance to aggressive corrosion environment.
The aim of this study was to investigate the welding seam surface properties of laser welded samples whose surfaces had either been and or not been subjected to Nd:YAG laser modification procedures with the help of SEM, elemental mapping, and AFM in addition to studying the microhardness of the AISI 316L stainless steel that had been joined by CO2 laser beam welding method.
2.1. Materials, welding procedure, and laser surface modification procedures
In this study, AISI 316L stainless steel, which is used in many branches of the industry, was used. Table 1 shows the chemical composition of AISI 316L stainless steel.
AISI 316L steel plates were butt joined without using any additional metal by means of a TRUMPF LASERCELL 1005 CO2 laser beam welding machine with 4 kW of power after being attached to the pre-prepared holding stand in line with the parameters given in Table 2. The CO2 laser beam welding method distinguishes itself from the traditional welding techniques because of its many characteristics such as low heat input, high concentration energy, high welding speed, narrow welding area, deep penetration, compatibility with automation, high mechanical strength, low distortion and the opportunity to weld without using welding wires [23-28].
Table 2. Welding parameters.
Laser power (W)
Travel speed (cm/min)
Shielding gas Gas flow rate (lt/min)
Focal length (mm)
Heat input (kJ/mm)
4000 180 50% Ar + 50% He 10 200 0.133
The laser surface modification procedures of the samples welded by CO2 laser beam welding were performed at the parameters specified in Table 3 by means of a micro scale power intensified Pulsed Nd:YAG laser, Rofin Tool Open brand laser welding machine with 150W. Overlapping seams were applied on all of the surfaces CO2 laser beam welded samples.
Table 3. The laser parameters used in laser surface modification.
Laser power (W) Travel speed (mm/s) Pulse duration (ms) Spot size (mm)
Shielding gas Gas flow rate (lt/min)
Heat input (kJ/mm)
50 5 5 0.7 Ar 12 0.1
100 5 5 0.7 Ar 12 0.2
150 5 5 0.7 Ar 12 0.3
2.2. Preparation of experimental samples and characterization procedures
100 ml pure H2O) that had been etched electrolytically by adding 200g load to the sinking end of a SHIMADZU brand measuring device. The surface roughness analysis was performed via a BRUKER AFM Q-SCOPE 250/400 brand device at a scanning size of 40μm and a scan rate of 0.5 Hz in tapping mode.
3. RESULTS AND DISCUSSION
3.1. The investigation of the welding area of the laser welded sample and the main material via AFM
Surface texture is an important topic in order to be able to understand the nature of material surfaces and plays an important role in the functional performance of many engineering components . Surface roughness is also a very important parameter for many applications. By characterizing surface roughness, we get information about which application areas that material can be used in effectively. The SEM image of the sample after the main material and welding seam surfaces of the sample, which had been joined by CO2 laser beam welding method, were polished with sandpaper is shown in Figure 1.
Figure 1. The SEM image of the samples before AFM characterization, a) main material surface, b) welding seam surface of the laser welded sample.
Figure 2. AFM image, a) main material surface b) welding seam surface.
3.2. SEM observations of the laser surface remelted and laser welded samples
Figure 3. The SEM image of the welding seam surface of the laser surface remelted and laser welded samples, a) 50W, b) 100W, c) 150W laser surface modification parameters.
The application of surface modification procedures on laser welded sample surfaces via Nd:YAG laser with micro scale power intensity allowed minimal heat input to the sample surfaces, and prevented loss of element in the welding areas. It can be said that since no elemental loss occurred on the welding surfaces of the samples, they can output the resistance expected of them in corrosive environments. Previous studies have indicated that the improvement in corrosion resistance with laser surface treatment of austenitic stainless steel [18,30,31]. The corrosion resistance of stainless steels mainly depends on the composition of the passive oxide layer characteristics on their surface. An increase chromium content in the passive oxide layer, cause a better resistance to corrosion of stainless steels. Researchers has been reported to laser surface treatments caused an increasing in Cr content and oxide layer thickness of laser treated surfaces . An increasing in Cr content and oxide layer thickness (mostly depends on the surface oxide film properties) ensures the corrosion resistance of stainless steel. In general, laser surface remelting (by using optimum laser process parameters) can lead to improvements in the corrosion behaviours, cavitation erosion resistance, tribological properties and biocompatibility (enhances adhesion, proliferation and spreading of cells on the laser treated surface of a biomaterial).
Figure 4. The results of the Elemental mapping of the welding seam surface of the laser surface remelted and laser welded samples, a) 50W, b) 100W, c) 150W laser surface modification parameters.
3.3. The AFM inspection of the laser surface remelted and laser welded samples
The average surface roughness values (Ra) of the laser welded samples, on whose surfaces laser modification had been applied, were identified via AFM analysis, and the obtained surface topography images are shown in Figure 6.
The Ra value obtained on the welding seam surface of the sample on which surface modification via 50W laser power had been applied was found to be 59.4nm, the Ra value obtained on the welding seam surface of the sample on which surface modification via 100W laser power had been applied was found to be 87.4nm, and the Ra value obtained on the welding seam surface of the sample on which surface modification via 150W laser power had been applied was found to be 224nm. It is clearly seen in the results that the roughness of sample surfaces increase significantly depending on the power of laser welding.
3.4. XRD inspection
The formations that could occur in the weld metal and HAZ regions of the laser welded sample and on the surface of the laser surface remelted and laser welded sample, were inspected be means of the XRD method in the 30o<2θ<105o interval, and the results are shown graphically in Figure 7.
Figure 7. XRD result, a) laser welded sample, b) laser surface remelted and laser welded sample
When the peaks of the main material and the peaks of the welded sample are compared on the graph (Figure 7a), it is seen that the peaks of the welded sample are sharper and more frequent, as well as increases in the peak intensities. This situation may be linked to the changes that occurred in the crystal lattice parameters of the sample due to heat input. Undesired formations such as chromium-carbide precipitation (M23C6) in the weld metal and HAZ were not observed in the XRD patterns.
3.5. Observations of microhardness
When the average microhardness distribution of welded joint was inspected, it was observed that the main material hardness value was 200 HV, HAZ hardness value was 225 HV, and weld metal hardness value was 240 HV, respectively. It is understood that the hardness values of HAZ and the weld metal are close to each other, and that the hardness value of the main material is a little lower. It is assumed that the reason the hardness of the weld metal is higher than that of the main material is related to the microstructure of the weld metal with fine grain size obtained as a result of the rapid cooling and solidifying due to the low heat input. In the literature, it is shown that the main reason that leads to hardness in weld metal is the fine grain size structure [24,32]. It can be concluded that heat input has no significant effect on the fact that the HAZ values of welded joint and the hardness value of the weld metal are very close to each other because, since austenitic stainless steel does not go through any phase transformation, hard phases such as martensite are not expected to form in their structures; therefore, their hardness values happen to be close to each other. Even though small increases may be seen during the inspection of the hardness of the laser welded samples on which laser surface modification had been applied, these increases did not lead to significant changes in the hardness, and hardness values similar to the samples with no laser modification were found. Since austenitic stainless steel cannot be hardened via heat treatment and since sample surfaces are exposed to micro scale laser beam at low powers, no significant changes in their hardness values occurred.
In this study, we analyzed the surface changes that were obtained after surface remelting procedure was applied on the surfaces of laser welded samples via Nd:YAG laser, as well as the microhardness of surface characterization of AISI 316L stainless steel joined by CO2 laser beam welding method, and the results are outlined below.
It was observed that the HAZ hardness values of the laser welded sample and the weld metal were close to each other, and that the hardness value of the main material was a little lower. No significant difference was found between the microhardness values of the laser welded sample and the laser welded sample on which laser surface modification was applied.
As a result of XRD inspection, while austenitic phase peaks were observed dominantly on the laser welded and non-laser welded samples on which no laser surface modification was applied, peak formations of δ-ferrite phase that prove the change in the crystallographic texture of the surface were observed in addition to the peak formations of austenitic phase. Also, undesired formations such as chromium-carbide precipitation (M23C6) in the laser welded samples with surface modification were not observed.
determined that the sample with the highest average surface roughness value was the laser welded sample on whose surface modification was applied via the highest laser power.
The author would like to express their thanks to Prof. Dr. Uğur Kölemen, and Dr. Fikret Yılmaz, Faculty of Arts and Sciences, Department of Physics, Gaziosmanpaşa University for the use of Atomic Force Microscope (AFM) equipment. The author would also like to thanks to KİTAM, Samsun Ondokuz Mayıs University for the use of SEM, XRD analysis.
1. M.B. Alexandru, C. Andrei, C. Marian, B. Zorica, R.C. Zizi, and S.E. Valentina, Stainless Steel the Environment Friendly Choice, Advances in Control, Chemical Engineering, Civil Engineering and Mechanical Engineering, Wseas Press, Spain (2010)
2. J.R. Davis, Introduction to Stainless Steels, Materials Park, Ohio, USA (2000)
3. J.R. Davis, ASM Speciality Handbook: Stainless steels, ASM International. Ohio, USA (1994) 4. R. Yılmaz, and M. Tümer, Int. J. Adv. Manuf. Technol., 67 (2013) 1433
5. D. Özyürek, Materials and Design, 29 (2008) 597
6. H.J. Cross, J. Beach, L.S. Levy, S. Sadhra, T. Sorahan, and C. McRoy, Manufacture, Processing and Use of Stainless Steel: A Review of the Health Effects, Prepared for Eurofer by the Institute of Occupational Health, University of Birmingham (1999)
7. A. Balamurugan, S. Rajeswari, G. Balossier, A.H.S. Rebelo, and J.M.F. Ferreira, Materials and Corrosion, 59 (2008) 855
8. C.T. Kwok, Laser Surface Modification of Alloys for Corrosion and Erosion Resistance, Woodhead Publishing in Materials, Cambridge, UK (2012)
9. J.J. Kim, and Y.M. Young, Int. J. Electrochem. Sci.,8 (2013) 11847
10.C.C. Shih, C.M. Shih, K.Y. Chou, S.J. Lin, and Y.Y. Su, Journal of Biomedical Materials Research Part A, 80 (2007) 861
11.D. Kuroda, S. Hiromoto, T. Hanawa, and Y. Katada, Materials Transactions, 43(2002) 3100 12.Y.C. Tang, S. Katsuma, S. Fujimoto, and S. Hiromoto, Acta Biomaterialia, 2 (2006) 709 13.A. Kurella, and N.B. Dahotre, Journal of Biomaterials Applications, 20 (2005) 5
14.E. Chikarakara, N. Sumsun, and B. Dermot, Applied Physics A: Materials Science & Processing, 101 (2010) 367
15.L. Hao, J. Lawrence, Y.F. Phua, G.C. Lim, and H.Y. Zheng, J Biomed Mater Res B Appl Biomater, 73(2005) 148
16.C.T. Kwok, F.T. Cheng, and H.C. Man, Materials Science and Engineering A, 290(2000) 55 17.S.H. Alavi, and S.P. Harimkar, Ultrasonics, 59 (2015) 21
18.W. Pacquentin, N. Caron, and R. Oltra, Applied Surface Science, 288 (2014) 34 19.E. Chikarakara, N. Sumsun, and B. Dermot, Applied Surface Science, 302 (2014) 321 20.H. Zhang, J. Han, Y. Sun, Y. Huang, and Zhou M, Materials Science and Engineering C, 56
21.R.K.Gupta, R. Sundar, B. Sunil Kumar, P. Ganesh, R. Kaul, K. Ranganathan, K.S. Bindra, V. Kain, S.M. Oak, and L.M. Kukreja, JMEPEG, 24 (2015) 2576
22.C.T. Kwok, K.H. Lo, W.K. Chan, F.T. Cheng, and H.C. Man, Corrosion Science, 53(2011) 1591 23.C. Köse, and R. Kaçar, Materials & Design, 64 (2014) 226
24.C. Köse, and R. Kaçar, Materials Testing, 56 (2014) 785
25.C. Köse, and R. Kaçar, Journal of the Faculty of Engineering and Architecture of Gazi University, 30 (2015) 235
27.C. Köse, and R. Kaçar, Int. J. Electrochem. Sci, 11 (2016) in press.
28.M. Taskin, U. Caligulu, and M. Turkmen, Materials Testing, 53 (2011) 741
29.R.R.L. De Oliveira, D.A.C. Albuquerque, T.G.S. Cruz, F.M. Yamaji, and F.L. Leite, INTECH Open Access Publisher (2012)
30.I.Y. Khalfallah, M.N. Rahoma, J.H. Abboud, and K.Y. Benyounis, Optics & Laser Technology, 43(2011) 806
31.O. Vedat Akgün, M. Üregen, and A.F. Çakir, Materials Science and Engineering: A, 203 (1995) 324
32.P. Sathiya, and M.Y. Abdul Jaleel,Optics and Lasers Technology, 42 (2010) 968